LMucko/crystallography-open-database huggingface dataset:
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 338 C Note: film 606
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012977
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 338 C
 Note: film 606
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5338
_cell_length_b                   3.5338
_cell_length_c                   3.5338
_cell_formula_units_Z            4
_cell_volume                     44.129
_database_code_amcsd             0014967
_diffrn_ambient_temperature      611.15
_exptl_crystal_density_diffrn    8.834
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012977
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 341 C Note: film 611
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012978
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 341 C
 Note: film 611
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5343
_cell_length_b                   3.5343
_cell_length_c                   3.5343
_cell_formula_units_Z            4
_cell_volume                     44.148
_database_code_amcsd             0014968
_diffrn_ambient_temperature      614.15
_exptl_crystal_density_diffrn    8.830
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012978
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 342 C Note: film 585
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012979
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 342 C
 Note: film 585
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5343
_cell_length_b                   3.5343
_cell_length_c                   3.5343
_cell_formula_units_Z            4
_cell_volume                     44.148
_database_code_amcsd             0014969
_diffrn_ambient_temperature      615.15
_exptl_crystal_density_diffrn    8.830
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012979
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 343 C Note: film 618
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012980
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 343 C
 Note: film 618
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5342
_cell_length_b                   3.5342
_cell_length_c                   3.5342
_cell_formula_units_Z            4
_cell_volume                     44.144
_database_code_amcsd             0014970
_diffrn_ambient_temperature      616.15
_exptl_crystal_density_diffrn    8.831
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012980
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 345 C Note: film 616 & 610
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012981
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 345 C
 Note: film 616 & 610
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5345
_cell_length_b                   3.5345
_cell_length_c                   3.5345
_cell_formula_units_Z            4
_cell_volume                     44.155
_database_code_amcsd             0014971
_diffrn_ambient_temperature      618.15
_exptl_crystal_density_diffrn    8.829
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012981
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 346 C Note: film 614
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012982
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 346 C
 Note: film 614
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5347
_cell_length_b                   3.5347
_cell_length_c                   3.5347
_cell_formula_units_Z            4
_cell_volume                     44.163
_database_code_amcsd             0014972
_diffrn_ambient_temperature      619.15
_exptl_crystal_density_diffrn    8.827
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012982
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 348 C Note: film 605
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012983
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 348 C
 Note: film 605
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5346
_cell_length_b                   3.5346
_cell_length_c                   3.5346
_cell_formula_units_Z            4
_cell_volume                     44.159
_database_code_amcsd             0014973
_diffrn_ambient_temperature      621.15
_exptl_crystal_density_diffrn    8.828
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012983
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 349 C Note: film 586
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012984
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 349 C
 Note: film 586
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5347
_cell_length_b                   3.5347
_cell_length_c                   3.5347
_cell_formula_units_Z            4
_cell_volume                     44.163
_database_code_amcsd             0014974
_diffrn_ambient_temperature      622.15
_exptl_crystal_density_diffrn    8.827
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012984
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 352 C Note: film 612
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012985
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 352 C
 Note: film 612
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5350
_cell_length_b                   3.5350
_cell_length_c                   3.5350
_cell_formula_units_Z            4
_cell_volume                     44.174
_database_code_amcsd             0014975
_diffrn_ambient_temperature      625.15
_exptl_crystal_density_diffrn    8.825
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012985
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 356 C Note: film 624
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012986
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 356 C
 Note: film 624
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5355
_cell_length_b                   3.5355
_cell_length_c                   3.5355
_cell_formula_units_Z            4
_cell_volume                     44.193
_database_code_amcsd             0014976
_diffrn_ambient_temperature      629.15
_exptl_crystal_density_diffrn    8.821
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012986
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 359 C Note: film 592
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012987
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 359 C
 Note: film 592
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5356
_cell_length_b                   3.5356
_cell_length_c                   3.5356
_cell_formula_units_Z            4
_cell_volume                     44.197
_database_code_amcsd             0014977
_diffrn_ambient_temperature      632.15
_exptl_crystal_density_diffrn    8.820
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012987
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 362 C Note: film 599
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012988
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 362 C
 Note: film 599
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5359
_cell_length_b                   3.5359
_cell_length_c                   3.5359
_cell_formula_units_Z            4
_cell_volume                     44.208
_database_code_amcsd             0014978
_diffrn_ambient_temperature      635.15
_exptl_crystal_density_diffrn    8.818
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012988
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 363 C Note: film 600
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012989
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 363 C
 Note: film 600
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5360
_cell_length_b                   3.5360
_cell_length_c                   3.5360
_cell_formula_units_Z            4
_cell_volume                     44.212
_database_code_amcsd             0014979
_diffrn_ambient_temperature      636.15
_exptl_crystal_density_diffrn    8.817
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012989
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 365 C Note: film 593
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012990
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 365 C
 Note: film 593
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5361
_cell_length_b                   3.5361
_cell_length_c                   3.5361
_cell_formula_units_Z            4
_cell_volume                     44.215
_database_code_amcsd             0014980
_diffrn_ambient_temperature      638.15
_exptl_crystal_density_diffrn    8.817
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012990
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 370 C Note: film 577 & 598
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012991
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 370 C
 Note: film 577 & 598
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5367
_cell_length_b                   3.5367
_cell_length_c                   3.5367
_cell_formula_units_Z            4
_cell_volume                     44.238
_database_code_amcsd             0014981
_diffrn_ambient_temperature      643.15
_exptl_crystal_density_diffrn    8.812
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012991
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 373 C Note: film 576
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012992
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 373 C
 Note: film 576
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5367
_cell_length_b                   3.5367
_cell_length_c                   3.5367
_cell_formula_units_Z            4
_cell_volume                     44.238
_database_code_amcsd             0014982
_diffrn_ambient_temperature      646.15
_exptl_crystal_density_diffrn    8.812
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012992
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 374 C Note: film 603
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012993
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 374 C
 Note: film 603
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5367
_cell_length_b                   3.5367
_cell_length_c                   3.5367
_cell_formula_units_Z            4
_cell_volume                     44.238
_database_code_amcsd             0014983
_diffrn_ambient_temperature      647.15
_exptl_crystal_density_diffrn    8.812
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012993
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 378 C Note: film 604
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012994
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 378 C
 Note: film 604
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5371
_cell_length_b                   3.5371
_cell_length_c                   3.5371
_cell_formula_units_Z            4
_cell_volume                     44.253
_database_code_amcsd             0014984
_diffrn_ambient_temperature      651.15
_exptl_crystal_density_diffrn    8.809
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012994
X-ray measurement of the thermal expansion of pure nickel Sample: at T = 388 C Note: film 589
Owen, E. A.; Yates, E. L.; Philosophical Magazine 21 (1936) 809–819; doi:

data_9012995
_publ_section_title
;
 X-ray measurement of the thermal expansion of pure nickel
 Sample: at T = 388 C
 Note: film 589
;
_journal_name_full               'Philosophical Magazine'
_journal_page_first              809
_journal_page_last               819
_journal_volume                  21
_journal_year                    1936
_chemical_compound_source        Synthetic
_chemical_formula_sum            Ni
_chemical_name_mineral           Nickel
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   3.5379
_cell_length_b                   3.5379
_cell_length_c                   3.5379
_cell_formula_units_Z            4
_cell_volume                     44.283
_database_code_amcsd             0014985
_diffrn_ambient_temperature      661.15
_exptl_crystal_density_diffrn    8.803
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_database_code               9012995